International Journal of Solids and Structures 6061 (2015) 107124
Contents lists available at ScienceDirect
International Journal of Solids and Structures
journal homepage: www.elsevier .com/locate / i jsols t r
Mechanical response of Ti6Al4V octet-truss lattice structures
http://dx.doi.org/10.1016/j.ijsolstr.2015.02.0200020-7683/ 2015 Elsevier Ltd. All rights reserved.
Corresponding author. Tel.: +1 434 982 5678.E-mail address: firstname.lastname@example.org (L. Dong).
Liang Dong a,, Vikram Deshpande b, Haydn Wadley aa Department of Materials Science and Engineering, University of Virginia, Charlottesville, VA 22903, United Statesb Engineering Department, Trumpington Street, University of Cambridge, UK
a r t i c l e i n f o a b s t r a c t
Article history:Received 11 December 2014Received in revised form 8 January 2015Available online 19 February 2015
Keywords:Octet-truss latticeElastic stiffnessStrengthTitanium alloys
A simple snap-fit and vacuum brazing method has been developed to fabricate three dimensional spacefilling octet-truss lattice structures from Ti6Al4V alloy sheets. Using strut lengths of 725 mm resultedin a relative density of the lattices ranging from 2% to 16%. The lattice elastic stiffness constants andstrengths have been characterized under through-thickness compression and in-plane shear as a functionof their relative density, and are shown to be well predicted by previously proposed micromechanicalmodels adapted to account for the increased nodal mass and strut separations of the snap-fit latticedesign. The Ti6Al4V octet-truss lattices exhibit excellent mechanical properties compared to othercellular material cell topology combinations, and appear to be promising candidates for high tem-perature applications where a robust mechanical performance is required.
2015 Elsevier Ltd. All rights reserved.
There are many ways to create 3D space filling cellular materials.Periodic cellular structures, are constructed from unit cells withhoneycomb (Bitzer, 1997; Wadley, 2003, 2006; Dharmasena,2008; Russell et al., 2008), tetrahedral (Sypeck, 2002; Kooistra,2004, 2007; Lim and Kang, 2006), 3D Kagome (Lim and Kang,2006; Lee et al., 2007; Park et al., 2011), octet truss (Bitzer, 1997;Fuller, 1961) and pyramidal (Kooistra, 2007; Queheillalt, 2005;Finnegan et al., 2007; Queheillalt et al., 2008) arrangements of websor struts. Tetrahedral, pyramidal and 3D Kagome unit cells requirestruts or webs to connect their out of plane members in order forthem to become statically determinant, stretch-dominated struc-tures (Deshpande et al., 2001). Space filling, structurally efficientlattices can then be constructed by the assembly of these unit cellsin three dimensions. These statically determinate lattice structurescan act as a material in the sense that their properties are indepen-dent of the size of the sample, provided its exterior dimensions arelarge compared to those of its cells. However, in some sandwichpanel applications (Sypeck, 2002; Kooistra, 2004, 2007; Wanget al., 2003) it may be preferable to use only the out of plane websor struts to maintain separation of the face sheets while utilizingthe faces to ensure unit cell static determinacy. Foams made frompolymers, metals or ceramics with interconnected or closed cellsalso provide a means for filling space with a random arrangementof cells (San Marchi et al., 2002). However, their cells have a vari-
able (but low) strut or web nodal connectivity, and are bendingdominated structures with moduli and strengths that decreaserapidly as the fraction of solid material (their relative density) isdecreased (Deshpande et al., 2001).
Lattice structures with open cell intermediate face sheetsbetween the layers of inclined struts, such as the octet-truss lattice(Bitzer, 1997; Fuller, 1961), have attracted considerable recentinterest since they are structurally more efficient than foams of asimilar density made from the same material. Recent castingapproaches have demonstrated the possibility of making octet-truss lattices with strut lengths in the 510 mm range(Deshpande et al., 2001), while self-propagating waveguide or laserbased stereo-lithographic methods, when combined with electro-less nickel plating or vapor deposition have enabled fabricationof micrometer scale structures (Torrents et al., 2012; Zheng et al.,2014; Bauer et al., 2014) offering opportunities to exploit otherfunctionalities of materials available in the small length scale limit.
An octet-truss lattice structure is illustrated in Fig. 1, and wasfirst proposed by Fuller (1961), as a method for filling 3D spacewith a structurally efficient truss structure of arbitrary cell size.Its nodes form a face centered cubic structure, Fig. 1(b). Since thestructure has a high nodal connectivity of 12, its mechanicalresponse is stretch-dominated (Deshpande et al., 2001). Whenmade from high specific modulus and strength materials, theoctet-truss lattice is therefore a weight efficient, stress supportingcellular topology, with a stiffness and strength predicted to scalelinearly with relative density, q (the density of the structure dividedby that of the material from which it is made) (Wadley, 2006).
Fig. 1. (a) An octet-truss lattice constructed by the 3D packing of unit cells. (b) A unit cell of the face centered cubic crystal symmetry octet-truss lattice is composed of acentral octahedral cell constructed with 12 struts that is bounded by 8 edge tetrahedrons. Each node within the octet lattice lies at the intersection of 12 struts.
Fig. 2. Material property charts comparing material stiffness (a) and strength (b) incompression against density. The experimental data (unit cell response, Table 2)and predicted range of these properties for the Ti6Al4V octet-truss latticestructure fabricated here (Ti6Al4V snap fit octet lattice) have been included forcomparison with other octet lattice truss materials. The grey shaded areas defineregions that cannot be reached under ambient conditions.
108 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
Material property charts are a useful way to compare themechanical properties of low density materials. Fig. 2 shows thedensity dependent modulus and strength under compressive load-ing for low density foams (polymer, metal and alumina) and spacefilling lattice structures made from investment cast Al7Si0.3Mg(Deshpande et al., 2001), Ti6Al4V and Ti6Al2Sn4Zr2Moalloys (Li et al., 2008a,b), similar structures made by electrodeposi-tion of Ni7P (Torrents et al., 2012; Zheng et al., 2014), from carbonfiber laminate composites (Cheung and Gershenfeld, 2013), photo-sensitive HDDA polymers (Zheng et al., 2014), and by the vapordeposition of alumina (Zheng et al., 2014; Bauer et al., 2014). Themoduli and strengths of both foams and lattices scale with thoseof the materials from which they are made (Gibson and Ashby,1999; Ashby, 2000), but foams are substantially more compliantand weaker than lattice topology counterparts (made with thesame density and material) for reasons identified above.
Octet-truss lattice structures made from low density metalalloys with strut diameters in the millimeter range are potentialcandidates for stress supporting aerospace applications. Light-weight aluminum alloy octet-truss lattice structures have beenmade by an investment casting (Deshpande et al., 2001) and by3D additive manufacturing methods (Rosen, 2007; Chu et al.,2010; Williams et al., 2011). However, these processes remain dif-ficult to implement with the highest strength to weight ratio alloysof aerospace interest. There is particular interest in making octet-truss structures from titanium alloys since their strength to weightratio is approximately twice that of aluminum alloys. Many titani-um alloys can also be used at continuous service temperatures wellabove the limits of other light metal alloys based on aluminum ormagnesium (Kulekci, 2008; Ye, 2003). Some titanium alloys alsohave excellent corrosion resistance, and are therefore widely usedin chemical processing equipment (Couper et al., 2009), and heatexchangers (Lu et al., 1998; Boomsma et al., 2003). The Ti6Al4V alloy is the most widely used titanium alloy, and accounts formore than 50% of total titanium usage. Its uses include aircraft tur-bine engine and structural components, fasteners, high perfor-mance automotive parts, and a variety of marine applications(Boyer et al., 1993; Ritchie et al., 1999; Brewer et al., 1998; Boyerand Briggs, 2005; Froes et al., 2004; Gorynin, 1999).
Titanium alloy lattice structures have been fabricated withaerospace-quality investment casting techniques (Li et al.,2008a,b). While this approach has the potential to enable fabrica-tion of complex shaped structures, it is costly to implement, andrequires development of methods to detect and repair the castingdefects often present in investment cast lattice structures (Wanget al., 2003). Because of the cost and complexity of the titaniuminvestment fabrication process, there is very limited mechanical
property data for titanium-based lattice structures as a functionof their relative density, Fig. 2.